Within the past 5 decades the use of ferroelectric composite made of ferroelectric ceramic immersed in polymer matrix has expanded significantly. One of the goals to embedding ceramic grains within a polymer matrix to form a 0-3 composite film is to combine the better properties of each phase, such as high piezoelectric activity of the ceramic and the mechanical resistance, formability and flexibility of the polymer, also because the 0-3 composite is the easier and cheaper way to fabricate this alternative electro-active material.
Some desirable properties for composite materials are: high piezoelectric charge and voltage coefficients for passive piezoelectric devices; large piezoelectric charge coefficient and low relative dielectric constant for active devices. Furthermore, the poling process of the composite film should be effective, which impose the composite must be homogeneously fabricated, i.e., the composite film should have uniformly dispersed ceramic grain.
Piezoelectric devices have some specific advantages over electromagnetic such as suitability to be miniaturized; there is no need of magnetic shielding; it is more efficient at least in the lower power range. There is a very large range of applications of piezoelectric materials, either as sensing element or as actuators. One of the most recent interests on piezoelectric materials is energy harvesting, converting mechanical to electrical energy. The aim of this research area is to provide clean energy attending the needs of the world in the fight against pollution.
Conventional ferroelectric materials such as lead zirconate titanate (PZT) [Jaffe 1969, Ren 2003, Klee 2010], modified lead titanate [Wang 2000, Chu 2004, Pontes 2001] and ferroelectric polymers [Lovinger 1983, Kawai 1969, Bauer 2000] have been used in applications which use either piezo or pyroelectric properties. Concerned to the piezoelectric applications, they have been employed in a large range of transducers such as for hydrophone [Lau 2002, Boumchedda 2007], dynamic strain measurements [Soman 2011], medical ultrasound [Zhang 2006, Muralt 2004] and non-destructive evaluation of structures [Brown 1996, Ciang 2008, Edwards 2006].
On the pyroelectric applications, ferroelectric materials can be used as infrared detectors [Sosnin 2000, Huang 2002, Guggilla 2006] and X-ray intensity measurements [De Paula 2005, Pontes 2010, De Carvalho 1997]. Using the pyroelectric property of the sensing element, KUBE Electronics AG (Switzerland) has developed a flame detection and gas analysis device [
Ferroelectric ceramics have high piezo and pyroelectric properties but, for some applications, their poor mechanical properties and the mismatch of the acoustic impedance with water and human tissue restrict their usage. On the other hand, ferroelectric polymers have mechanical flexibility and formability but their piezo and pyroelectric activity are low. To overcome these problems composite materials made of ferroelectric ceramic and polymer have been investigated as an alternative material which combine the better properties of ceramic and polymer [Furukawa 1976, Dias 1996, Sakamoto 2006, Wong 2006, Kumar 2005, Estevam 2011, Feng 2010].
According to Newnham and co-workers [Newnham 1978] there are ten connectivity patterns in which a two phase composite system can be fabricated, ranging from unconnected 0-0 pattern to a 3-3 pattern in which both phases are three dimensionally self-connected. The easier and cheaper composite to obtain is the 0-3 pattern, that means the ceramic grains are dispersed (unconnected) into a polymer matrix (self-connected three dimensionally). The main goal of embedding ferroelectric ceramic grains within a polymer matrix is to obtain a material which displays the combined better properties of each single phase. However it is very difficult to obtain a 0-3 composite with high ceramic content. There are basically two problems: high ceramic content will provide a mixed connectivity due to the percolation of the grains; high ceramic concentration means low flexibility of the composite material.
But these problems have not drawn the interest of researchers in using the 0-3 composite, on the contrary, it intensified the search for optimum results and many studies on the polarization of the composites have been conducted [Furukawa 1986, Lau 2007, Ploss 2001, Wong 2002]. Still seeking a more effective polarization of the composite material, studies with the inclusion of a semiconductor phase were carried out [Sa-Gong 1986, Sakamoto 2002, Renxin 2006, Ploss 2006, Chau 2007]. These efforts were not in vain and 0-3 composites are being used as sensors and transducers, and is now a well-established alternative to conventional ferroelectric materials for many applications. New methods of preparing ferroelectric ceramics have also been studied and the latest is the hydrothermal method for obtaining ceramic powder [Shimomura 1991, Morita 2010]. The grain size and structure are also objects of study.
This work presents the preparation and characterization of PZT ceramic obtained by different methods. The influence of the synthesis method on the grain size and the morphology are also object of study. The fabrication and characterization of composite films with 0-3 connectivity, immersing nanoparticles of PZT into the non-polar poly(vinylidene fluoride) – PVDF as the polymer matrix were presented. For comparison there are some results obtained with composite samples made of ceramic particles recovered with a conducting polymer and also using the conducting polymer as a third phase. Moreover it presents the results obtained with the new material that includes a semiconductor phase, polyaniline – PAni as a sensing material and as a piezoelectric material for energy harvesting. In this sample the PZT grain was partially covered by PAni, which allowed better distribution of grains in the polymer matrix in comparison with the inclusion of the 3rd phase separately, avoiding a continuous electrical flux path which does not allow the polarization process of the composite sample. The use of this composite as sensor and power converter is an indicative that it is a good alternative for technological applications.
The control of some parameters is important to achieve the desired properties in lead zirconate titanate (PZT) materials. These parameters include the absence of intermediate crystalline phases, a defined and fixed stoichiometry, as well as a homogeneous distribution of lead in the material. Lead zirconate titanate (PZT) is a very interesting ceramic that has good piezoelectric properties used to making ultrasonic transducers, filters and pyroelectric detectors [Haertling 1999]. This material can be prepared using different ways but the most important is using low temperature to obtain the crystalline phase. This condition promotes the homogeneous lead distribution and consequently occurs the formation of pure phase PZT. The presence of secondary phases reduces the dielectric and piezoelectric constants [Zaghete 1999, Zaghete 1992]. To minimize theses problems some chemicals processes has been proposed as the optional procedure. Methods such as sol-gel [Ishikawa 1994], hydrothermal synthesis [Pan 2007, Abothu 1999] and Pechini's method [Zaghete 1992] can be used.
It is known that ceramic materials prepared from chemical solutions routes are transformed via a nucleation and growth process, often requiring high temperatures to surmount the large energy barriers of the nucleation and growth of the stable phase. Consequently, these energy barriers frequently determine the calcinations conditions and therefore the characteristics such as, particle size, morphology and degree of aggregation of the precursor powder. The most significant advance in this field, however, consists of the ability to control phase development at low calcinations temperatures to avoid lead evaporation.
The expected phase equilibrium (perovskite) may grow starting from a gel matrix under a nucleus along a certain crystallographic orientation. This type of heterogeneous nucleation eliminates the need for the system to exceed the activation energy required to form the nucleus, as in the case of systems with homogeneous nucleation. As a result, the perovskite phase may crystallize at lower temperatures.
The present study show the influence of synthesis method on size and morphologic distribution of particle and the amount of perovskits phase synthesized at different temperatures. The procedure of PZT synthesis, based on Pechini’s method [Zaghete 1992] makes use of the capability that certain α-hydroxycarboxylic organic acids possess of forming polybasic acid chelates with several cations. When mixing with a polyhydroxylic alcohol and heating, the chelate transforms into a polymer, maintaining the cations homogeneously distributed.
The organic part is eliminated at low temperatures forming reactive oxides with well-controlled stoichiometry. Pure PZT with composition Pb(Zr0.48Ti0.52)O3 can be prepared from the metal-citrate complex polyesterified in ethylene glycol. Appropriate quantities of Zr, Ti and Pb solutions were mixed and homogenized by stirring at 90ºC for 3 h. Next, the temperature was increased to 130-140ºC, yielding a high viscous polyester resin. The powder was calcined at 600, 700 and 800ºC for 2h and ball milled for 2h in isopropylic alcohol medium.
Recently, the hydrothermal synthesis has been widely used in the study of these materials for the production of particles with nanometric sizes, high purity and crystallinity, good stoichiometric control and good yield. There are few reports relating to the study on the PZT synthesized by the hydrothermal method in literature. In one of these works, PZT powder was obtained with cubic morphology and crystalline phase by hydrothermal synthesis [PAN 2007]. By controlling the variables process of the synthesis, it becomes possible to change the morphology, the particle size, as well as the hydrothermal synthesis assisted by microwave method that has the advantage of producing rapid heating, thereby promoting homogeneous nucleation of particles [Moreira 2009, Rao 1999].
Hydrothermal media provide an effective reaction environment for the synthesis of numerous ceramic materials because of the combined effects of solvent, temperature, and pressure on ionic reaction equilibrium. The conventional hydrothermal method has become an effective synthetic route in Materials science by dramatically increasing the control of the micro/nanometric morphology and orientation [LUO 2008]. In addition, this method is environmentally friendly and depends on the solubility of the chemical salts in water under temperature and pressure conditions.
The key factors in this method are the vapor pressure and solubility of the chemical salts in water [Lencka 1995]. In contrast to the conventional hydrothermal method which requires a long time typically several days and high electric power (over thousand watts) [Dutta 1994], microwave-assisted heating is a greener approach to synthesize materials within a shorter time typically several minutes to some few hours less than the duration of the conventional method and with lower energy consumption (hundreds of watts).
The desired PZT product can be synthesized using Pb(NO3)2, ZrOCl2.8H2O, TiO2, KOH. At first, a suspension containing ZrOC2.8H2O, Pb(NO3)2 and TiO2 was prepared in aqueous medium. After that, KOH aqueous solution containing 3.31g of KOH (1.84 mol.L-1, pH=14). was add to the precursor suspension and then kept at room temperature under stirring for approximately 20 minutes. It was further placed containing all the reagents in Teflon jars, sealed and taken to the microwave for the synthesis of PZT powder.
The synthesis temperature was 180ºC and the lower time used to obtain PZT was 0.5 hour, under constant pressure of approximately 10 Bar. The PZT powders were synthesized using microwave-assisted hydrothermal digester (MARS CEM, USA). The precursor was further again loaded into a 90 mL Tefflon autoclave reaching 30% of its volume. The autoclave was sealed and placed into a microwave-assisted hydrothermal system using 2.45 GHz microwave radiation with a maximum output power of 800 W. Then the solid product was washed with distilled water until a neutral pH was obtained and was further dried at room temperature.
The obtained powders were characterized by X-ray powder diffraction using a Rigaku, DMax 2500PC with rotator anode at 50 kV and 150 mA, Cu Kα radiation in the 2θ range from 20º to 80º with 0.02ºmin-1. A field emission gun scanning electron microscope (SEM-FEG)-ZEISS SUPRA 35 microscope was used to analyze the shape and size of particles; energy dispersive X-ray microanalysis spectroscopy (EDS) was used for compositional determination. All measurements were taken at room temperature.
Today it is well known the effectiveness of the synthesis rote on the perovskits phase formation but it isn't well understood the influence of the particle size on the composite properties. Some of results obtained for PZT prepared by pechini´s method and synthesis hydrothermal assisted by microwave were presented to show the different characteristic as function of the synthesis way.
The analysis of the crystal structure of the material indicated mixture of the tetragonal and rhombohedral phase that is characteristics of the morphotropic phase transition region (YU 2007) Figure 1. When prepared by the Pechini’s method has been the formation of pure crystalline phase from 600ºC, the same result can be observed with hydrothermal treatment at 180ºC for 1 hour. Also is possible to observe that the distribution of particle size and average particle size are directly affected by the temperature of thermal treatment as well as by the synthesis process, Figures 2 and 3. The purity of the composition was analyzed by EDS and found a homogeneous distribution of Pb, Ti, Zr on the surface of the entire sample as showed in Figure 4.
2.2. Polymer matrix
Poly(vinylidene fluoride) (PVDF) is a thermoplastic with excellent mechanical, optical and thermal properties, and showing resistance to attack of various chemicals [Lovinger 1982]. Formed by repeated units of (-H2C-CF2-)n, has a molecular weight around 105 g / mol. Depending on the means of acquiring or thermal history, PVDF can possess the degree of crystallinity from 45 to 60%, melting temperature (Tm) in the range from 165 to 179ºC and glass transition temperature (Tg) of about -34ºC. Its crystal structure is spherulitic (composed of lamellar crystalline radial). The range of relatively low melting temperature and some properties of the polymer described above ensure easy processing by melting and blending, which means great advantage in large scale production. The PVDF can also be processed by casting that may result in thin films.
Relative to the molecular structure, PVDF is a linear polymer that has permanent electric dipoles approximately perpendicular to the direction of their chains. These dipoles are formed by the electronegativity difference between atoms of hydrogen and fluorine. PVDF can be found in four distinct structural phases α, β, γ and δ.α phase is the most common, this being non-polar usually obtained by cooling molten. The β phase (polar) is very attractive technical-scientific because of its piezoelectric and pyroelectric activity.
2.3. Getting PZT grains coated with PAni
The monomer aniline (C6H5NH2) was purchased from Sigma-Aldrich and used in the synthesis after vacuum distillation. For the polymerization of aniline was employed oxidant ammonium persulfate from MERCK. To obtain the PZT particles partially coated with polyaniline, the PZT powder was incorporated into the solution of aniline and 1M cloridric acid under stirring at a temperature around 2ºC for approximately 2 h. The solution was filtered and washed with 0.1M hydrochloric acid and the product was dried in an oven at 50ºC for 3h.
Figure 5 shows the FEG-SEM micrograph of (a) the PZT and (b) PAni-coated PZT particles. It can be seen the lack of smooth of the coated-particle surface.
The PVDF in the form of powder was mixed with pure PZT, the PZT particles coated with PAni and PAni and PZT placed separately. The mixtures were then placed between sheets of Kapton and pressed close to the melting temperature of PVDF. To find the optimum condition for preparation of the composite film the effect of pressing temperature, time and pressure to be taken by the mixtures were studied.The optimum conditions were found to be: temperature of 185ºC for about 1 minute at a pressure of about 7.6 MPa. The thickness of the films was in the range from 100 to 420 μm depending on the ceramic content. The composite films were obtained with different volume fractions of ceramic, which was calculated using the equation below [Marin-Franch 2002]:
where m is the mass and ρ is the density. The subscript c and p are related to ceramic and polymer, respectively. Φc is the volume fraction of ceramic. Figure 6 shows FEG images of the composite sample. It can be seen the homogeneous distribution of the ceramic nanoparticles recovered with PAni.
The protonation degree of polyaniline can be controlled so that the conductivity of the composite, i. e, their permittivity can be changed and facilitate the polarization process [Wei 2007, Wong 2005, Or 2003, Zhou 2005]. Pani can have its conductivity controlled by the pH [Blinova 2008], which means that in more acidic - pH below 4.0 - it begins to undergo the process of doping and its conductivity gradually increased with decreasing pH.
3. Characterization of the composite
Aluminum electrodes with 1.0 cm of diameter were vacuum evaporated onto both sides of the sample for electrical contact. The composite films were poled with several electric field strengths and times in silicone oil bath with controlled temperature. A TREK high voltage power supply was used for the dc poling process. The dielectric data were taken using an impedance analyzer HP 4192 A in circular samples with 1.5 cm diameter.
An important aspect to note in materials is its electrical response when subjected to an alternating electric field. So it can be observed by measuring the impedance spectroscopy the behavior of dielectric constant versus frequency. Figure 7 shows the behavior of the real relative permittivity ε' and loss factor ε” which have their highest values with the preparation of PZT-PAni at lower pH values, and in ε" this increase is more significant. This is also an indication that the conductivity σ of the material increases, since it is directly related to the permittivity ε of the material by the relationship [Poon 2004]:
where ω is the angular frequency of an external electric field applied and ε0 is the electric permittivity in vacuum. In systems which contain grains covered with PAni doped partially or completely, ε' and especially ε'' reach high values at lower frequencies, and for these cases the magnitude of ε'' is bigger than ε', indicating high charge mobility, characteristics of the polymeric phase.
The piezoelectric activity of the composite films was studied by measuring the longitudinal piezoelectric coefficient
The longitudinal piezoelectric coefficient
By means of thermally stimulated depolarization current (TSDC) is possible to obtain the pyroelectric coefficient p(T). However it is necessary to clean up this curve, or leave it free from unwanted effects, such as the fluctuation of space charges injected during the polarization, since the interest is only the dipolar contribution, because it will remain even after heating the sample, if the provided temperature does not exceed the bias.
Figure 9 shows that for the first heating the depolarization current is greater than for the next heat, in which current tends to stabilize. This stabilized curve is the pyroelectric current, i.e., that due to dipolar relaxation.
|Composites||Volumetric fraction of ceramic (%)|
|PSTM/PEKK [PELAIZ-BARRANCO 2005]||50||21|
|PTCa/PEKK [PELAIZ-BARRANCO 2005]||50||28|
|PZT/PU with 1% of graphite (SAKAMOTO 2001)||49||13|
|PZT/PVC [LIU 2006]||30||6|
|PZT/PVC [LIU 2006]||50||17|
|PZT/PVDF with 10% of PAni [RENXIN 2006]||50||28|
|PZT-PAni/PVDF redoped in pH=3.7||30||15-20*|
The pyroelectric coefficient p(T) can be obtained using the equation below:
where P is the polarization, A the area of the electrode, Ip the pyroelectric current and dT/dt the heating rate. Figure 10 shows the pyroelectric coefficient as a function of the temperature for different composites with 30 vol.% of PZT.
It can be observed low values of pyroelectric coefficient for composites PZT-PAni/PVDF fully doped (Δ). This effect is expected, since its polarization is hindered by the high conductivity of the films. For the composites PZT/PVDF and PZT-PAni/PVDF dedoped in the range of 0 to 40oC the behavior of the pyroelectric coefficients are similar, while the composite PZT-PAni/PVDF redoped (pH 3.7) has larger values. At temperatures above 40ºC, the composite with PAni dedoped has little increase in pyroelectric coefficient with increasing temperature, while the composites PZT/PVDF and PZT-PAni/PVDF redoped having similar behavior, suffer a sharp increase. Table 2 shows the value of pyroelectric coefficient at room temperature for some composite materials. The composite with ceramic particle partially covered with PAni after suitable protonation degree display pyroelectric coefficient comparable with composite samples described in literature, which uses high ceramic volume fraction.
|Composite||Volumetric fraction of ceramic (%)||p(T) (μC.m-2.oC-1)|
|PZT/Epoxy [DAS-GUPTA 1999]||40||40|
|BaTiO3/rubber [DAS-GUPTA 1999]||30||60|
|TGS/PVDF [DAS-GUPTA 1999]||80||90|
|PT/PVDF [DAS-GUPTA 1999]||62||130|
|PZT/PVDF [DAS-GUPTA 1999]||50||10|
|PTCa/P(VDF-TrFE) [DAS-GUPTA 1999]||65||130|
|PZT-PAni/PVDF redoped in pH=3.7||30||70|
4. On the energy conversion
For material to be used as a sensor, the relationship between output voltage and input power should be linear, i.e., the responsivity should remain constant. And regarding the magnitude of responsivity, it may indicate the quality of the sensor, i.e. the larger the magnitude, more input signal is being converted into output signal.
Four samples: two of PZT/PVDF 30/70 vol%, one previously polarized with a electric field of 10 MV/m for 1 hour and another with a field of 5 MV/m for 15 minutes, a PZT/PVDF 50/50 vol% polarized with 10 MV/m for 1 hour, and one of PAni with 30/70 vol% PZT-PAni/PVDF redoped at pH 3.7 and polarized with 5 MV/m for 15 minutes were compared. Figure 11 illustrates the behavior of the output voltage as a function of frequency and input power.
A close analysis of the results allows observing that the composite with polyaniline was superior in all respects in comparison to the other composites. Although the PZT/PVDF 50/50 vol% has close values of output voltage (Figure 11), the electric field and the time spent to polarize it were high. Furthermore, the ferroelectric ceramics content is higher. Without conducting phase in the composite the poling conditions have to be actually higher for the best properties of electroactivity. It can easily be observed when comparing the two composites PZT/PVDF 30/70 in volume. The composite polarized with higher electric field and spending more time showed higher output voltage. Yet comparing the composites with 30% load PZT or PZT-PAni, the latest presents better results.
In photopyroelectricity the upper face of the sample is painted with black ink to optimize the energy absorption. Since the sample works as a thermal transducer, absorbed modulated radiation increases the temperature of the sample and the heat is transformed into an electrical signal generated by the potential difference between the two faces of the sample. According to Mandelis and Zver [Mandelis 1985] the photopyroelectric voltage (V(ω)) can be written, for the optically opaque and thermally thick pyroelectric sample, as:
is the amplitude, η is quantum efficiency, I0 is the light intensity, F is the thermal coefficient which depends on the thermal parameters of the sample, ω is the angular frequency of light modulation, αs is the thermal diffusivity of the sample, Ls the thickness and φ is the phase of the photopyroelectric signal. In the amplitude p is the pyroelectric coefficient, ε0 the vacuum permittivity and κ the relative permittivity.
The concept of energy harvesting must be related to capture the ambient energy and convert it into usable electrical energy without environment attack i.e., a clean electric energy. Although there are a number of sources of harvestable ambient energy, such as solar energy and energy from wind [Schwede 2010, Chang 2002], piezoelectric materials are very interesting due to their ability to convert applied strain energy into usable electric energy. Some countries are working hard on it and Israel, for example, using piezoelectric plates under the track, can obtain power enough to provide electricity to a medium house.
The energy recovery from the wasted energy used or not was a topic of discussion for a long time. Unused energy exists in various forms, such as vibration, water, wind, sun, heat, cold, human and vehicle movement, and shock waves. In today's world, there is a strong technological breakthrough in the way of life. More and more people are carrying portable electronic devices. These devices have and enable incredible power and versatility in communication and problem-solving. But as the technologies of portable computers and microcontrollers have grown tremendously, the battery energy and the storage technology did not follow them. New technology allows these portable devices become ever smaller, but the sizes of cells or batteries are still the same and the limited operating life is a great problem.
An alternative to the batteries and cells is the implementation of a method to obtain energy surrounding devices that could power supply them. Piezoelectric materials can be used to convert mechanical energy into electrical energy that can be used to power other devices. Energy harvesting using piezoelectric materials have attracted many attention of the researchers around the world. Many works have been published in this area [Koyama 2009, Umeda 1997, Sodano 2004, Zheng 2009, Wang 2010, Anton 2007] and the focus is to find a material which gives power enough to allow its use commercially.
The cantilever beam structure is one commum setup for energy harvesting. It uses PZT thin film to transforme the mechanical vibration into electrical energy. In the present work composite films were put under a track which will simulates car traffic or people movement. Within this context, four square composite samples with 4.5 cm2 were poled with suitable electric field and copper foil (1 mm thick) was glued for electrical contact as show in Figure 12. Table 3 shows the longitudinal
To evaluate the power generated by these samples, they were pressed by the blue car continuosly as shown in Figure 13. The weight and the frequency of the blue car which will impact the composite samples can be controlled and fixed during the experiment. The output voltage provided by the piezoelectric composite can be measured with an oscilloscope.
A track is project and constructed with two parts. A bottom steel base with electrical tape on its top, fixed to a press device plane. A top made of aluminum with the bottom with duct tape, and attached to external screws that make this part of mobile resource, since the composite is between bottoms and top part of the track it receives the impact of the track above it. The composites were used as transducer individually, in series and in parallel. Then they were connected directly (open circuit) to acquire the waveforms from the digital oscilloscope. Further, the composites were connected in circuit (closed circuit) with the oscilloscope at the entrance acquiring waveforms again. Finally, voltages were measured at the capacitors for every minute during 10 minutes. Acquisition board was used to get the electrical signal provided by the composite. This board consists of a retifier circuit AC/DC and a output capacitor.
The experiments starts using a force of 200 kgf, to stroke the composites with a frequency of 3.0 Hz, and a capacitor of 3300 μF. The open circuit (directly on the composites) and the closed circuit measurements for each composite, and combined composites in parallel (//) which are showed in Figure 14.
Experimental results show that an open circuit output voltage of 17.0 Vpp are generated while in closed circuit the peak to peak voltage generated is 2.13 V because of the impedance of the capacitor.
Figure 15 shows the energy analysis of the experiments for different configurations of the composite films. It can be seen the increasing energy supplied when the composite films are connected in parallel. The useful energy, after 10 min, by four composite films is about ten times higher than the energy generated by one composite film. The values of energy in Figure 15 were calculated from the measurement of the output voltage against time, using the following relation:
where U is the available energy and V is the voltage measured on the capacitor. The voltage was measured during the charge of the capacitor due to the deformation of the composite films by the applied stress.
Composite films made of PZT ceramic immersed in PVDF polymer matrix were obtained with 0-3 connectivity. The method of synthesis can provide different structure of the ceramic and also can provide ceramic particles with different size distribution which are important parameters for the electroactive properties of the sample. The inclusion of a semiconductor phase, separately or coating the ceramic particles improve the poling process of the composite, avoiding timing consuming and high applied electric field to polarize the ferroelectric ceramic particles immerse into the polymer matrix. The advantages of recovered particles is the better control of the homogeneity of the particle distribution avoiding percolation of conductive particles that may form a continuous path which not allow the poling process.
Using small amount of ceramic (30 vol%) the composite was used as infrared detector, indicating the possibility of its use as intruder detector or fire alarm. Using the right protonation (doping) degree of the PAni, the composite display piezo and pyroelectric coefficients high as many composite materials with higher ceramic content even when poled with lower electric field and shorter poling time. The study of energy harvesting simulating people walking or vehicle traffic showed low power generated by each small composite sample (4.5 cm2 area) but the association of four samples enhanced the converted electrical energy from the energy wasted during vehicle traffic. These preliminary results show that the composite material deserves to be deeply studied as alternative material to obtain clean energy.
This work has financial support from the Brazilian Agencies: Fundação de Amparo à Pesquisa do Estado de São Paulo – FAPESP and Conselho Nacional de Desenvolvimento Científico e Tecnológico – CNPq through the Instituto Nacional de Ciência e Tecnologia de Materiais em Nanotecnologia – INCTMN.
Abothu I. R. et al. 1999Processing of Pb(Zr0.52Ti0.48)O3 (PZT) ceramics from microwave and conventional hydrothermal powders. , 34, (9), 1411-1419.
Anton S. R. Sodano H. A. 2007A review of power harvesting using piezoelectric materials (2003- 2006), ., 16, R 1R21.
Bauer F. 2000PVDF shock sensors: applications to polar materials and high explosives, , 47 (6), 1448 EOF 54 EOF
Blinova N. V. et al. 2008Control of polyaniline conductivity and contact angles by partial protonation, . 57 66 69
Boumchedda K. Hamadi M. Fantozzi G. 2007Properties of a hydrophone produced with porous PZT ceramic, ., 27 4169 4171
Brown L. F. Mason J. L. 1996Disposable PVDF Ultrasonic Transducers for Nondestructive Testing Applications, , 43 (4), 560- 567.
Chang L. 2002Wind energy conversion systems, , 12 16
Chau K. H. Wong Y. W. Shin F. G. 2007Enhancement of piezoelectric and pyroelectric properties of composite films using polymer electrolyte matrix, ., 91, 252910 EOF
Chu-Y S. Chen-Y T. 2004Fabrication of modified lead titanate piezoceramics with zero temperature coefficient and its application on SAW devices, ., 51 (6), 663 EOF 7 EOF
Ciang C. C. Lee-R J. Bang-J H. 2008Structural health monitoring for a wind turbine system: a review of damage detection methods, . 19, 122001 EOF
Das-Gupta D. K. 1999Ferroelectric composite sensor materials, ., 10 (2), 97 EOF 126 EOF
De Carvalho A. A. Alter A. J. 1997Measurement of X-ray intensity in the medical diagnostic range by a ferroelectric detector, , 44 (6), 1198 EOF 1203 EOF
De Paula M. H. et al. 2005Microcontrolled pyroelectric instrument for measuring X-ray intensity in mammography, ., 43 751 755
Dias C. J. Das-Gupta D. K. 1996Inorganic ceramic/polymer ferroelectric composite electrets, ., 3 (5), 706 EOF 734 EOF
Dutta P. K. et al. 1994Hydrothermal Synthesis and Dielectric Properties of Tetragonal BaTiO3, ., 6 9 1542 1548
Edwards G. et al. 2006PMN-PT single-crystal transducer for non-destructive evaluation, , 132 434 440
Estevam G. P. De Melo W. L. B. Sakamoto W. K. 2011Photopyroelectric response of PTCa/PEEK composite, , 82, 023903.
Feng Y. et al. 2010A model for 0 3piezoelectric composites with an interlayer, , 1922- 1927.
Furukawa T. Fujino K. Fukada E. 1976Electromechanical properties in the composites of epoxy resin and PZT ceramics, 15 (11), 2119 EOF 2129 EOF
Furukawa T. Suzuki K. Date M. 1986Switching process in composite systems of PZT ceramics and polymers, , 68 33 44
Guggilla P. et al. 2006Pyroelectric ceramics for infrared detection applications, 60 1937 1942
Haertling G. H. 1999Ferroelectric ceramics: history and technology, , 82, (4), 797 EOF 818 EOF
Huang Z. et al. 2002Infrared optical properties of PbTiO3 ferroelectric thin films, J., 35 246 248
Ishikawa K. et al. 1994Crystallization and growth process of lead titanate fine particles from alkoxide-prepared powders, . 33, 3495 EOF 3499 EOF
Jaffe, H., Piezoelectric applications of ferroelectrics, IEEE Trans.Electr. Devices, 16 (6), 544- 554 ( 1969
Kawai H. 1969The piezoelectricity of poly(vinylidene fluoride), ., 8 975 976
Klee M. et al. 2010Ferroelectric and piezoelectric thin films and their applications for integrated capacitors, piezoelectric ultrasound transducers and piezoelectric switches, IOP Conf. Series: . 8, 012008 EOF
Koyama D. Nakamura K. 2009Array configurations for higher power generation in piezoelectric energy harvesting, , 1973 1976
Kumar N. Nath R. 2005Ferroelectric phase stability studies in potassium nitrate: Polyvinylidene fluoride composite films, ., 97, 0 24105 EOF
Lau S. T. et al. 2002Piezoelectric composite hydrophone array, 96 14 20
Lau S. T. et al. 2007A poling study of lead zirconate titanate/polyurethane 0 3composites, ., 102, 044104.
Lencka M. M. Riman R. E. 1995Thermodynamics of the Hydrothermal Synthesis of Calcium Titanate with Reference to Other Alkaline-Earth Titanates, ., 7 18 25
Liu-F X. et al. 2006Piezoelectric and dielectric properties of PZT/PVC and graphite doped with PZT/PVC composites, , 127 261 266
Lovinger A. 1982, D. C. Basset Ed., Applied Science Publishers, 195 273London.
Lovinger A. 1983Ferroelectric Polymers, , 220 1115 1121
Luo Z. et al. 2008Self-assembly of BaMoO4 single-crystalline nanosheets into microspheres, , 110 17 20
Mandelis A. Zver M. M. 1985Theory of photopyroelectric spectroscopy of solids, ., 57 (9), 4421- 4430.
Marin-Franch P. et al. 2002PTCa/PEKK piezo-composites for acoustic emission detection, , 99 236
Moreira M. L. et al. 2009Synthesis of Fine Micro-sized BaZrO3 Powders Based on a Decaoctahedron Shape by the Microwave-Assisted Hydrothermal Method, , 833 839
Morita T. 2010Piezoelectric Materials Synthesized by the Hydrothermal Method and Their Applications, , 3 5236 5245
Muralt P. Baborowski J. 2004Micromachined Ultrasonic Transducers and Acoustic Sensors Based on Piezoelectric Thin Films, , 12 101 108
Newnham R. E. Skinner D. P. Cross L. E. 1978Connectivity and piezoelectric-pyroelectric composites, , 13 525 536
Or Y. et al. 2003Modeling of poling, piezoelectric, and pyroelectric properties of ferroelectric 0 3composites, . 94 (5).
Pan Q. et al. 2007Intense blue-light emission from hydrothermally synthesized lead zirconate titanate platelets. , 61, (4-5), 1210 EOF 1213 EOF
Pelaiz-Barranco A. Marin-Franch P. 2005Piezo- pyro, ferro-, and dielectric properties of ceramic/polymer composites obtained from two modifications of lead titanate, ., 97 03411 034414
Ploss B. Kopf S. 2006Improving the pyroelectric coefficient of ceramic/polymer composite by doping the polymer matrix, , 338 145 151
Ploss B. et al. 2001Poling study of PZT/P(VDF-TrFE) composites, , 61 957 962
Pontes D. S. L. et al. 2001Microstructural, dielectric and ferroelectric properties of calcium-modified lead titanate thin films derived by chemical processes, , 21 1107 1114
Pontes W. et al. 2010PZT, for measuring energy fluence rate of X-ray used in superficial câncer therapy, ., 38 210 219
Poon Y. M. Shin F. G. 2004A simple explicit formula for the effective dielectric constant of binary 0-3 composites, ., 39 1277 1281
Rao K. J. et al. 1999Synthesis of Inorganic Solids Using Microwaves, Chem. Mater., 11 882 895
Ren-L T. et.al 2003Piezoelectric and ferroelectric films for microelectronic applications, . B 99 159 163
Renxin X. et al. 2006Dielectric and piezoelectric properties of 0 3PZT/PVDF composite doped with polyaniline, ., 21 (1), 84- 87.
Sa-Gong et. al 1986Poling flexible piezoelectric composites, , 5, 13’- 142.
Sakamoto W. K. De Souza E. Das-Gupta D. K. 2001Electroactive properties of flexible piezoelectric composites, , 4 (3), 201 EOF 204 EOF
Sakamoto W. K. et al. 2006PTCa/PEEK composite acoustic emission sensors, ., 13 (5), 1177 EOF 1182 EOF
Sakamoto W. K. Marin-Franch P. Das-Gupta D. K. 2002Characterization and application of PZT/PU and graphite doped PZT/PU composite, , 100 165 174
Schwede J. W. et al. 2010Photon-enhanced thermionic emisión for solar concentrador Systems, , 9 762 767
Shimomura K. et al. 1991Preparation of lead zirconate titanate thin film by hydrothermal method, ., 30 2174 2177
Sodano H. A. Park G. Inman D. J. 2004Estimation of electric charge output for piezoelectric energy harvesting, , 40 49 58
Soman J. O’Neal C. B. 2011Fabrication and Testing of a PZT Strain Sensor for Soil Applications, , 11 (1), 78 EOF 85 EOF
Sosnin A. 2000Image infrared converters based on ferroelectric-semiconductor thin-layer systems, , 3 (4), 489 EOF 495 EOF
Umeda M. Nakamura K. Ueha S. 1997Energy storage characteristics of a piezo-generator using impact induced vibration, ., 36 3146 3151
Wang C. M. et al. 2000Calcium modified lead titanate thin films for pyroelectric applications, , 2
Wang-A D. Ko-H H. 2010Piezoelectric energy harvesting from flow-induced vibration, . 20, 025019 EOF
Wei N. et al. 2007Effect of electrical conductivity on the polarization behaviour and pyroelectric, piezoelectric property prediction of 0-3 ferroelectric composites, ., 40 2716 2722
Wong C. K. Shin F. G. 2006Effect of electrical conductivity on poling and the dielectric, pyroelectric and piezoelectric properties of ferroelectric 0-3 composites, ., 41 229 249
Wong C. K. Shin F. G. 2005Electrical conductivity enhanced dielectric and piezoelectric properties of ferroelectric 0 3composites, J. Appl. Phys.
Wong C. K. Wong Y. W. Shin F. G. 2002Effect of interfacial charge on polarization switching of lead zirconate titanate particles in lead zirconate titanate/polyurethane composites,., 92 (7), 3974 EOF
Yu N. Zakharov A. V. Borodin Borodin V. Z. 2007Pyroelectric properties of PZT-type ferroelectric ceramics in the morphotropic phase-transition region,, 71, (5), 709-710.
Zaghete M. A. et al. 1999The Effect of Isostructural Seeding on the Microstructure and Piezoelectric Properties of PZT Ceramics, , 25,. 239 244
Zaghete M. A. et al. 1992Phases Characterization In PZT Obtained From Organic Solutions Of Citrates. , 75 2088 2093
Zhang Q. Q. et al. 2006High frequency broadband PZT thick film ultrasonic transducer for medical imaging applications, 44, e 711e715.
Zheng B. Chang-J C. Gea H. C. 2009Topology optimization of energy harvesting devices using piezoelectric materials, ., 38 17 23
Zhou Y. et al. 2005Effects of polarization and permittivity gradients and other parameters on the anomalous vertical shift behavior of graded ferroelectric thin films, ., 98, 034105 EOF